Polycarbonates (PC) are a group of thermoplastic polymers containing carbonate groups in their chemical structures. Polycarbonates used in engineering are strong, tough materials, and some grades are optically transparent. They are easily worked, molded, and thermoformed. Because of these properties, polycarbonates find many applications. Polycarbonates do not have a unique resin identification code (RIC) and are identified as "Other", 7 on the RIC list.
Repeating chemical structure unit of
Polycarbonate made from bisphenol A
|Density (?)||1.20-1.22 g/cm3|
|Abbe number (V)||34.0|
|Refractive index (n)||1.584-1.586|
|Limiting oxygen index||25-27%|
|Water absorption--Equilibrium (ASTM)||0.16-0.35%|
|Water absorption--over 24 hours||0.1%|
|Ultraviolet (1-380 nm) resistance||Fair|
|Young's modulus (E)||2.0-2.4 GPa|
|Tensile strength (?t)||55-75 MPa|
|Elongation (?) at break||80-150%|
|Compressive strength (?c)||>80 MPa|
|Poisson's ratio (?)||0.37|
|Izod impact strength||600-850 J/m|
|Notch test||20-35 kJ/m2|
|Abrasive resistance ASTM D1044||10-15 mg/1000 cycles|
|Coefficient of friction (?)||0.31|
|Speed of sound||2270 m/s|
|Glass transition temperature (Tg)||147 °C (297 °F)|
|Heat deflection temperature|
|Vicat softening point at 50 N||145-150 °C (293-302 °F)|
|Upper working temperature||115-130 °C (239-266 °F)|
|Lower working temperature||-40 °C (-40 °F)|
|Thermal conductivity (k) at 23 °C||0.19-0.22 W/(m·K)|
|Thermal diffusivity (a) at 25 °C||0.144 mm²/s|
|Linear thermal expansion coefficient (?)||65-70 × 10-6/K|
|Specific heat capacity (c)||1.2-1.3 kJ/(kg·K)|
|Dielectric constant (?r) at 1 MHz||2.9|
|Permittivity (?)||2.568 × 10-11F/m|
|Relative permeability (?r) at 1 MHz||0.866(2)|
|Permeability (?) at 1 MHz||1.089(2) ?N/A2|
|Dissipation factor at 1 MHz||0.01|
|Volume resistivity (?)||1012-1014?·m|
|Greases and oils||Good-fair|
|Gas permeation at 20 °C|
|Carbon dioxide||400-800 cm3·mm/(m2·day·Bar)|
|Water vapour||1-2 gram·mm/(m2·day) @ 85%-0% RH gradient|
Polycarbonates received their name because they are polymers containing carbonate groups (-O-(C=O)-O-). A balance of useful features, including temperature resistance, impact resistance and optical properties, positions polycarbonates between commodity plastics and engineering plastics.
In this way, approximately one billion kilograms (one million tonnes) of polycarbonate is produced annually. Many other diols have been tested in place of bisphenol A (e.g., 1,1-bis(4-hydroxyphenyl)cyclohexane and dihydroxybenzophenone). The cyclohexane is used as a comonomer to suppress crystallisation tendency of the BPA-derived product. Tetrabromobisphenol A is used to enhance fire resistance. Tetramethylcyclobutanediol has been developed as a replacement for BPA.
The ring-opening polymerization of cyclic carbonates has been investigated.
Polycarbonate is a durable material. Although it has high impact-resistance, it has low scratch-resistance. Therefore, a hard coating is applied to polycarbonate eyewear lenses and polycarbonate exterior automotive components. The characteristics of polycarbonate compare to those of polymethyl methacrylate (PMMA, acrylic), but polycarbonate is stronger and will hold up longer to extreme temperature. Polycarbonate is highly transparent to visible light, with better light transmission than many kinds of glass.
Polycarbonate has a glass transition temperature of about 147 °C (297 °F; 420 K), so it softens gradually above this point and flows above about 155 °C (311 °F; 428 K). Tools must be held at high temperatures, generally above 80 °C (176 °F; 353 K) to make strain-free and stress-free products. Low molecular mass grades are easier to mold than higher grades, but their strength is lower as a result. The toughest grades have the highest molecular mass, but are much more difficult to process.
Unlike most thermoplastics, polycarbonate can undergo large plastic deformations without cracking or breaking. As a result, it can be processed and formed at room temperature using sheet metal techniques, such as bending on a brake. Even for sharp angle bends with a tight radius, heating may not be necessary. This makes it valuable in prototyping applications where transparent or electrically non-conductive parts are needed, which cannot be made from sheet metal. PMMA/Acrylic, which is similar in appearance to polycarbonate, is brittle and cannot be bent at room temperature.
Main transformation techniques for polycarbonate resins:
Polycarbonate is mainly used for electronic applications that capitalize on its collective safety features. Being a good electrical insulator and having heat-resistant and flame-retardant properties, it is used in various products associated with electrical and telecommunications hardware. It can also serve as a dielectric in high-stability capacitors. However, commercial manufacture of polycarbonate capacitors mostly stopped after sole manufacturer Bayer AG stopped making capacitor-grade polycarbonate film at the end of year 2000.
The second largest consumer of polycarbonates is the construction industry, e.g. for domelights, flat or curved glazing, and sound walls, which all use extruded flat solid or multiwall sheet, or corrugated sheet.
A major application of polycarbonate is the production of Compact Discs, DVDs, and Blu-ray Discs. These discs are produced by injection molding polycarbonate into a mold cavity that has on one side a metal stamper containing a negative image of the disc data, while the other mold side is a mirrored surface.
In the automotive industry, injection-molded polycarbonate can produce very smooth surfaces that make it well-suited for sputter deposition or evaporation deposition of aluminium without the need for a base-coat. Decorative bezels and optical reflectors are commonly made of polycarbonate. Due to its low weight and high impact resistance, polycarbonate is the dominant material for making automotive headlamp lenses. However, automotive headlamps require outer surface coatings because of its low scratch resistance and susceptibility to ultraviolet degradation (yellowing). The use of polycarbonate in automotive applications is limited to low stress applications. Stress from fasteners, plastic welding and molding render polycarbonate susceptible to stress corrosion cracking when it comes in contact with certain accelerants such as salt water and plastisol. It can be laminated to make bullet-proof "glass", although "bullet-resistant" is more accurate for the thinner windows, such as are used in bullet-resistant windows in automobiles. The thicker barriers of transparent plastic used in teller's windows and barriers in banks are also polycarbonate.
The third generation Mazda MX-5 was offered with a Power Retractable Hard Top (PRHT) variant that uses a folding hardtop made of polycarbonate, which added only 36 kg (79 lb) to the weight of a comparably equipped soft top without diminishing trunk space when retracted.
So-called "theft-proof" large plastic packaging for smaller items, which cannot be opened by hand, is uniformly made from polycarbonate.
Polycarbonate, being a versatile material with attractive processing and physical properties, has attracted myriad smaller applications. The use of injection molded drinking bottles, glasses and food containers is common, but the use of BPA in the manufacture of polycarbonate has stirred serious controversy (see Potential hazards in food contact applications), leading to development and use of "BPA-free" plastics in various formulations.
Polycarbonate is commonly used in eye protection, as well as in other projectile-resistant viewing and lighting applications that would normally indicate the use of glass, but require much higher impact-resistance. Polycarbonate lenses also protect the eye from UV light. Many kinds of lenses are manufactured from polycarbonate, including automotive headlamp lenses, lighting lenses, sunglass/eyeglass lenses, swimming goggles and SCUBA masks, and safety glasses/goggles/visors including visors in sporting helmets/masks and police riot gear (helmet visors, riot shields, etc.). Windscreens in small motorized vehicles are commonly made of polycarbonate, such as for motorcycles, ATVs, golf carts, and small planes and helicopters.
Typical products of sheet/film production include applications in advertisement (signs, displays, poster protection). But also applications as automotive safety glazing (ECE R 43).
The light weight of polycarbonate as opposed to glass has led to development of electronic display screens that replace glass with polycarbonate, for use in mobile and portable devices. Such displays include newer e-ink and some LCD screens, though CRT, plasma screen and other LCD technologies generally still require glass for its higher melting temperature and its ability to be etched in finer detail.
As more and more governments are restricting the use of glass in pubs and clubs due to the increased incidence of glassings, polycarbonate glasses are becoming popular for serving alcohol because of their strength, durability, and glass-like feel.
Other miscellaneous items include durable, lightweight luggage, MP3/digital audio player cases, ocarinas, computer cases, fountain pens, riot shields, instrument panels, tealight candle containers and blender jars. Many toys and hobby items are made from polycarbonate parts, like fins, gyro mounts, and flybar locks in radio-controlled helicopters, and transparent LEGO (ABS is used for opaque pieces).
Standard polycarbonate resins are not suitable for long term exposure to UV radiation. To overcome this the primary resin can have UV stabilisers added. These grades are sold as UV stabilized polycarbonate to injection moulding and extrusion companies. Other applications including polycarbonate sheet may have the anti-UV layer added as a special coating or a coextrusion for enhanced weathering resistance.
Polycarbonate is also used as a printing substrate for nameplates and other forms of industrial grade under printed products. The polycarbonate provides a barrier to wear, elements, and fading.
Polycarbonate has been used in artistic applications. American pop artist Roy Lichtenstein used a polycarbonate-based, thermoplastic film called Rowlux in his work, including pieces in his portfolio 10 Landscapes  and Moonscape. 
Many polycarbonate grades are used in medical applications and comply with both ISO 10993-1 and USP Class VI standards (occasionally referred to as PC-ISO). Class VI is the most stringent of the six USP ratings. These grades can be sterilized using steam at 120 °C, gamma radiation, or by the ethylene oxide (EtO) method. However, scientific research indicates possible problems with biocompatibility. Dow Chemical strictly limits all its plastics with regard to medical applications. More recently, scientists at the IBM Almaden Research Center have developed aliphatic polycarbonates with improved biocompatibility and degradability for nanomedicine applications.
Some major smartphone manufacturers use polycarbonate. Nokia has used polycarbonate-base in their phones starting with the N9's unibody case in 2011. This practice continues with various phones in the Lumia series. Samsung has started using polycarbonate with Galaxy S III's battery cover in 2012 and this practice continues with various other phones in the Galaxy series. Apple started using polycarbonate with the iPhone 5C's unibody case in 2013.
In 1953, Hermann Schnell at Bayer in Uerdingen, Germany patented the first linear polycarbonate. The brand name "Merlon" was registered in 1955, and later changed to Makrolon in the 1980s. Also in 1953, one week after the patent was submitted by Bayer, Daniel Fox at General Electric in Schenectady, New York, independently submitted a closely related patent on a branched polycarbonate. Both companies filed for U.S. patents in 1955, and agreed that the company lacking priority would be granted a license to the technology. Once patent priority was resolved in Bayer's favor, Bayer began commercial production under the trade name Merlon in 1958 and GE began production under the name Lexan in 1960. The production of Lexan was taken over by SABIC in 2007. There are many applications for the LEXAN polycarbonate. One of them is patented production of the motorcycle helmets that meet the worldwide safety standards and requirements for this type of safety equipment. Their patented innovative Vision Protection System (VPS) is specific treatment of polycarbonate that makes it fog- and scratch-resistant.
After 1970, the brownish original polycarbonate tint was improved to "glass-clear".
The use of polycarbonate containers for the purpose of food storage is controversial. The basis of this controversy is that hydrolysis (degradation by water, either by leaching or at high temperature) releases bisphenol A (BPA):
More than 100 studies have explored the bioactivity of bisphenol A derived from polycarbonates. Bisphenol A appeared to be released from polycarbonate animal cages into water at room temperature and it may have been responsible for enlargement of the reproductive organs of female mice. However, the animal cages used in the research were fabricated from industrial grade polycarbonate, rather than FDA food grade polycarbonate.
An analysis of the literature on bisphenol A leachate low-dose effects by vom Saal and Hughes published in August 2005 seems to have found a suggestive correlation between the source of funding and the conclusion drawn. Industry-funded studies tend to find no significant effects whereas government-funded studies tend to find significant effects.
Sodium hypochlorite bleach and other alkali cleaners catalyze the release of the bisphenol A from polycarbonate containers.Alcohol is one recommended organic solvent for cleaning grease and oils from polycarbonate.
Studies have shown that at high temperatures between 70 and 80 °C and high humidity, polycarbonates hydrolyzes to bisphenol A (BPA). This condition is similar to that observed in most incinerators. After about 30 days under such conditions, surface crystals were formed. Measurements indicated that about 70% by mass of the surface crystals were bisphenol A (BPA). BPA is a compound that is currently on the list of potential environmental hazardous chemicals. It is on the watch list of many countries, such as United States and Germany.
The leaching of BPA from polycarbonate can also occur at environmental temperature and normal pH (in landfills). The amount of leaching increases as the material becomes older. A study found that the decomposition of BPA in landfills (under anaerobic conditions) does not occur. It will therefore be persistent in landfills. Eventually, it will find its way into water bodies and contribute to aquatic pollution.
In the presence of UV light, oxidation of this polymer yields compounds such as ketones, phenols, o-phenoxybenzoic acid, benzyl alcohol and other unsaturated compounds. This has been suggested through kinetic and spectral studies. The yellow color formed after long exposure to sun can also be related to further oxidation of phenolic end group
This product can be further oxidized to form smaller unsaturated compounds. This can proceed by two different pathways, the products formed depends on which mechanism takes place.
Photo-aging is another degradation route for polycarbonates. Polycarbonate molecules (such as the aromatic ring) absorb UV radiation. This absorbed energy causes cleavage of covalent bonds, which initiates the photo-aging process. The reaction can be propagated by side chain oxidation, ring oxidation or photo-fries rearrangement. Products formed include phenyl salicylate, dihydroxybenzophenone groups, and hydroxydiphenyl ether groups.
Polycarbonate phenyl salicylate 2,2-dihydroxybenzophenone
Waste polycarbonate will degrade at high temperatures to form solid, liquid and gaseous pollutants. A study showed that the products were, by mass, about 40-50% liquid, 14-16% gases, while 34-43% remained as solid residue. Liquid products contained mainly phenol derivatives (~75%) and bisphenol (~10%) also present. This is of concern when incinerating optical data disks.
Phenol derivatives are environmental pollutants, classified as volatile organic compounds (VOC). Studies show that they are likely to facilitate ground-level ozone formation and increase photo-chemical smog. In aquatic bodies, they can potentially accumulate in organisms. They are persistent in landfills, do not readily evaporate and would remain in the atmosphere.
Polycarbonate can satisfactorily be given a single-dose sterilization exposure (22) but tends to become brittle much above 2.5 Mrad.CS1 maint: multiple names: authors list (link)